Journal of Power Sources 97±98 (2001) 240±243
Nanomaterial-based Li-ion battery electrodes Naichao Lia, Charles R. Martina,*, Bruno Scrosatib a
Department of Chemistry, University of Florida, Gainesville, FL 32611, USA b Department of Chemistry, University ``La Sapienza'', 00185 Rome, Italy Received 6 June 2000; accepted 19 January 2001
Abstract We have been exploring the use of the template method to prepare nanostructured Li-ion battery electrodes. These nanostructured electrodes show improved rate capabilities relative to thin-®lm control electrodes prepared from the same material. In this paper we discuss nanostructured Sn-based anodes. Li-ion battery anodes derived from oxides of tin have been of considerable recent interest because they can, in principle, store over twice as much Li as graphite. However, large volume changes occur when Li is inserted and removed from these Sn-based materials, and this causes internal damage to the electrode resulting in loss of capacity and rechargability. We describe here a new nanostructured SnO2-based electrode that has extraordinary rate capabilities, can deliver very high capacities (e.g. >700 mAh g 1 at 88C), and still retain the ability to be discharged and recharged through as many as 800 cycles. These electrodes, prepared via the template method, consist of monodisperse 110 nm-diameter SnO2 nano®bers protruding from a current-collector surface like the bristles of a brush. The dramatically-improved rate and cycling performance is related to the small size of the nano®bers that make up the electrode and the small domain size of the Sn grains within the nano®bers. # 2001 Elsevier Science B.V. All rights reserved. Keywords: Fibres; Electrode; Li-ion battery; Electrode; Nanomaterials
Lithium-ion batteries are becoming the power sources of choice for modern consumer electronic devices [1±6]. Although, commercially available, these batteries are still the subject of intense research activity aimed at the development of new high-performance electrode and electrolyte materials. Research on alternative anodes focuses on materials that have higher Li storage capacities than the carbonaceous materials (e.g. graphite) currently employed. Anodes derived from oxides of tin (e.g. SnO2) have been of considerable recent interest because they can, in principle, store over twice as much Li as graphite [7,8]. However, large volume changes occur when Li is inserted and removed from these Sn-based materials, and this causes internal damage to the electrode resulting in loss of capacity and rechargeability [9±11]. Prior work has shown that both the size of the particles making up the electrode, and the size of the grains within these particles, play critical roles in this unwanted decomposition process, speci®cally, electrodes composed of smaller particles and grains show better cyclability [9,12]. This suggests that combining basic research efforts in nanomaterials and Sn-based electrodes might yield better anode * Corresponding author. E-mail address: [email protected]
materials for Li-ion batteries. We describe here a new nanostructured SnO2-based electrode that can deliver very high capacity (>700 mAh g 1) at very high discharge currents, and still retain the ability to be discharged and recharged through many cycles. The Li electrochemistry of the SnO2-based electrodes is interesting because it entails ®rst the irreversible conversion of the tin oxide to metallic tin 4Li 4e SnO2 ) 2Li2 O Sn
and then the reversible alloying/dealloying of the Sn with Li  xLi xe Sn , Lix Sn;
0 x 4:4
It is this alloying/dealloying process that gives this material its charge storage capacity. In theory as many as 4.4 Li atoms can be stored per atom of Sn which would give this anode a maximum theoretical charge storage capacity of 781 mAh g 1 versus 372 mAh g 1 for graphite. In addition, this charge is stored at high energies, within one volt of the reduction potential for Li to Li metal. However, as noted above, Sn undergoes dramatic volume changes (up to 300%) upon formation of the Li±Sn alloy, which results in internal damage and loss of capacity with cycling [9±11].
0378-7753/01/$ ± see front matter # 2001 Elsevier Science B.V. All rights reserved. PII: S 0 3 7 8 - 7 7 5 3 ( 0 1 ) 0 0 7 6 0 - 1
N. Li et al. / Journal of Power Sources 97±98 (2001) 240±243
We have previously shown that the template method [13,14] can be used to prepare electrodes that consist of nano®bers or nanotubules of Li insertion materials that protrude from an underlying current collector surface like the bristles of a brush [15±20]. These nanostructured electrodes show vastly superior rate capabilities relative to control electrodes prepared from the same materials. The template method is a general approach for preparing
nanomaterials that entails synthesizing the desired material within the pores of a microporous membrane or other solid [13±20]. The membranes employed contain cylindrical pores with monodisperse diameters, and corresponding cylindrical nanostructures are obtained. In this case, a microporous polycarbonate ®lter (Poretics) was used as the template; this membrane had a nominal pore diameter (supplied by the manufacturer) of 50 nm and a pore density
Fig. 1. (A) Scanning electron micrograph of the nanostructured SnO2 electrode. The nanofibers are protruding from an underlying Pt current-collector surface; (B) Transmission electron micrograph of a single SnO2 nanofiber before electrochemical cycling.
N. Li et al. / Journal of Power Sources 97±98 (2001) 240±243
of 6 108 pores per cm2 of membrane surface area. A solution-based method was used to deposit the cylindrical SnO2 nano®bers within the pores of this membrane. The membrane was immersed for 24 h into a solution consisting of 0.338 g SnCl22H2O, 0.03 ml 37% HCl, and 0.47 ml ethyl alcohol and then applied to the surface of a Pt foil current collector. The solvent was removed at 808C in air, and the template membrane was burnt away using an oxygen plasma. This left nano®bers of a tin oxide precursor material which was heated at 4408C in air to convert them into crystalline SnO2 (cassiterite, as proven by X-ray diffraction) nano®bers. Electron microscopic analyses (Fig. 1) showed that these nano®bers were 110 nm in diameter, 6.0 mm in length (thickness of template), and that there were 5 108 nano®bers per cm2 of current collector surface. As discussed previously,  it is typically the case that the nano®bers obtained have larger diameters than the nominal pore diameter of the template membrane. From the diameter, density, and length of the nano®bers it is easy to show that these electrodes have 10 cm2 of SnO2 area per cm2 of substrate electrode area. A thin-®lm control electrode was prepared by doing the same synthesis on a Pt current collected without using the polycarbonate template membrane. This electrode contained the same quantity of SnO2 (0.081 mg) as the nanostructured electrode. Electron microscopic analysis showed that this ®lm was 550 nm in thickness. Electrochemical experiments were conducted in a threeelectrode cell using either the nanostructured or thin-®lm SnO2 as the working electrode and Li foils as the counter and reference electrodes. The electrolyte was 1 M LiClO4 in a 30:70 (vol.%) mixture of ethylene carbonate and diethyl carbonate. The reversible capacity was measured by conducting constant current charge/discharge experiments between potential limits of 0.2 and 0.9 V versus Li/Li. Prior to charge/discharge experiments, the electrodes were charged from the open circuit potential (2.5 V) to the lower potential limit of 0.2 V, then discharged back to the upper limit of 0.9 V. The results of these experiments are summarized in Fig. 2. At very low discharge rates both the nanostructured and thin-®lm control electrodes show experimental capacities that are essentially identical. As is always observed, [10,15±20] capacity falls off with increasing discharge rate, however, the extent of capacity loss is dramatically reduced for the nanostructured electrode. Fig. 3 compares the discharge capacity versus the number of charge/discharge cycles for the nanostructured and control electrodes. There is absolutely no loss of capacity with cycling for the nanostructured electrode, indeed there is a slight increase in capacity with increasing cycle number. We have now cycled nanostructured electrodes through 800 cycles; the capacity ultimately stabilizes and no further increase is observed. We are currently investigating this interesting result of increasing capacity with increased cycle number. In contrast, the thin-®lm control electrode shows a decay in capacity with cycling (Fig. 3). The charging and
Fig. 2. Discharge capacity vs. charge/discharge rate for the nanostructured and thin-film control electrodes. From reference 20; used with permission.
discharging were done at a very high rate, 88C, which corresponds to a current density of 0.32 mA cm 2. In spite of this high rate, the capacity of the nanostructured electrode is still large, >700 mAh g 1. This, again, emphasizes the extraordinary rate capabilities of this electrode. The coulombic ef®ciency was 97%. This paper has shown that combining basic research efforts in nanomaterials and Sn-based anodes could lead the way to the development of a new class of nanostructured anodes for Li-ion batteries. It is clear, however, that much additional research will be required before practical nanostructured anodes will be developed. It is of interest to note that another report on nanostructured Sn electrodes (prepared via a different route) has recently appeared, however, these electrodes showed poor cyclability and rate capabilities . Other approaches for preparing microstructured electrode materials have been described [22±24]. The extended cycle life of our template-prepared electrodes is undoubtedly related to the small size [9,12] of the nano®bers
Fig. 3. Capacity vs. cycle number for the nanostructured and thin-film control electrodes at a charge/discharge rate of 88C over the potential window of 0.2±0.9 V. From reference 20; used with permission.
N. Li et al. / Journal of Power Sources 97±98 (2001) 240±243
that make up the electrode. In addition, Fig. 1B shows that the nano®bers are composed of very small grains of electrode material, which has also been shown to be bene®cial to the cycle life of these materials. A detailed study of the properties and characteristics of the nanostructured SnO2 electrodes is currently underway. Acknowledgements This work was supported by the U.S. Department of Energy. References       
B. Scrosati, Nature 373 (1995) 557. O. Oyama, T. Tatsuma, T. Sotomura, Nature 373 (1995) 598. A.R. Armstrong, P.G. Bruce, Nature 381 (1996) 499. J.R. Dahn, T. Zheng, Y. Liu, J.S. Xue, Science 270 (1995) 590. R. Koksbang, J. Baker, H. Shi, M.Y. Saidi, Solid State Ion. 84 (1996) 1. S. Megahed, B. Scrosati, Interface 4 (1995) 34. K. Tahara, H. Ishikawa, F. Iwasaki, S.S. Yahagi, A. Sakkata, T. Sakai, Eur. Pat. Appl. 93111938, 1993, p. 2.
 Y. Idota, T. Kubota, A. Matsufuji, Y. Maekawa, T. Miyasaki, Science 276 (1997) 1395.  J.O. Besenhard, J. Yang, M. Winter, J. Power Sources 68 (1997) 87.  T. Brousse, R. Retoux, D. Schleich, J. Electrochem. Soc. 145 (1998) 1.  I.A. Courtney, J.R. Dahn, J. Electrochem. Soc. 144 (1997) 2045.  I.A. Courtney, J.R. Dahn, J. Electrochem. Soc. 144 (1997) 2943.  J.C. Hulteen, C.R. Martin, J. Mater. Chem. 7 (1997) 1075.  C.R. Martin, Science 266 (1994) 1961.  G. Che, K.B. Jirage, E.R. Fisher, C.R. Martin, H. Yoneyama, J. Electrochem. Soc. 144 (1997) 4296.  C.J. Patrissi, C.R. Martin, J. Electrochem. Soc. 146 (1999) 3176.  M. Nishizawa, K. Maukai, S. Kuwabata, C.R. Martin, H. Yoneyama, J. Electrochem. Soc. 144 (1997) 1923.  G. Che, B.B. Lakshmi, E.R. Fisher, C.R. Martin, Nature 393 (1998) 346.  N. Li, C.J. Patrissi, G. Che, C.R. Martin, J. Electrochem. Soc. 197 (2000) 2044.  N. Li, C.R. Martin, B. Scrosati, Electrochem. Solid-State Letters 3 (2000) 316.  A.H. Whitehead, J.M. Elliott, J.R. Owen, J. Power Sources 81/82 (1999) 33±38.  J.O. Besenhard, M. Hess, J. Huslage, K. Jurewicz, U. Krebber, J. Power Sources 43/44 (1993) 493.  J. Yang, M. Winter, J.O. Besenhard, Solid State Ion. 90 (1996) 281.  A. L Tipton, S. Passerini, B.B. Owens, W.H. Smyrl, J. Electrochem. Soc. 143 (1996) 3473.